- NANO EXPRESS
- Open Access
Collision-spike Sputtering of Au Nanoparticles
© Sandoval and Urbassek; licensee Springer. 2015
- Received: 10 March 2015
- Accepted: 8 July 2015
- Published: 6 August 2015
Ion irradiation of nanoparticles leads to enhanced sputter yields if the nanoparticle size is of the order of the ion penetration depth. While this feature is reasonably well understood for collision-cascade sputtering, we explore it in the regime of collision-spike sputtering using molecular-dynamics simulation. For the particular case of 200-keV Xe bombardment of Au particles, we show that collision spikes lead to abundant sputtering with an average yield of 397 ± 121 atoms compared to only 116 ± 48 atoms for a bulk Au target. Only around 31 % of the impact energy remains in the nanoparticles after impact; the remainder is transported away by the transmitted projectile and the ejecta. The sputter yield of supported nanoparticles is estimated to be around 80 % of that of free nanoparticles due to the suppression of forward sputtering.
- Molecular dynamics
Ion irradiation of constrained systems, such as nanoparticles (NPs), nanostructured surfaces, or two-dimensional systems, has recently received increased interest . Ion impact of NPs finds applications in the sputtering of aerosols  and in the irradiation of dust particles in space or in a plasma environment [3, 4]. In addition, dedicated experiments have become possible where NPs are supported on a surface and irradiated by an ion beam. Such experiments allow to modify the NPs [5, 6] and also to measure the sputter yield by monitoring the size change of the NP as a function of ion dose. Such experiments have been performed by Klimmer et al.  (Ziemann, P. Private communication 2010. Unpublished) and more recently by Greaves et al. . Yang et al.  determined the sputter yield of Au NPs in the size range of 10–100 nm under 20-keV C 60 impact.
From the theoretical point of view, sputtering of spherical NPs has been studied most extensively. Molecular dynamics (MD) computer simulation can shed light on this phenomenon. Many previous simulations focused on Au targets and studied exemplary cases, such as 100-keV Au → Au (sphere radius R=4 nm) [9, 10] or 16- and 64-keV Au → Au (R=10 nm) . Järvi et al. [12, 13] analyzed the sputtering of Au NPs with radii up to 8 nm by 25-keV Ga ions using MD computer simulation.
Sputtering of NPs by collision cascades can be investigated by analytical theory and—relatively inexpensive—Monte Carlo simulations; in this area, rather encompassing studies have been carried out. Nietiadi et al. carried out an extensive simulation study of the sputter yield as a function of sphere radius R [14, 15], using both Monte Carlo and exemplary MD simulations. Their study focused on 20-keV Ar impacts on amorphous Si spheres; here, sputtering proceeds mostly by the ballistic collision-cascade mechanism , and the contribution of collision spikes is minor. They showed that sputtering has a maximum as a function of sphere size when the ion penetration depth is of the order of the sphere radius; these results corroborate the earlier findings of Järvi et al. [12, 13]. In a recent publication, Urbassek et al.  extended these collision-cascade results to arbitrarily shaped NPs.
Greaves et al.  present experiments and accompanying computer simulations for the sputter yield enhancement during the bombardment of Au nanorods under 80-keV Xe irradiation. They show strong enhancements of the sputter yield compared to the sputtering of a bulk Au target and emphasize the role of cluster emission for high-yield events and of channeling for low-yield events.
Here, we analyze the sputtering of spherical Au NPs of radius R=12.4 nm by 200-keV ion impact. This system corresponds to the experimental study of Klimmer et al.  (Ziemann, P. Private communication 2010. Unpublished) who investigated the burrowing of supported NPs into the substrate under continuous ion irradiation. Since this is a clear case of spike sputtering, MD is used for simulation. We demonstrate the large variety of sputter events occurring. The sputter yield of supported NPs will be smaller than that of free NPs due to the suppression of forward sputtering.
Using MD simulation, we study the sputtering of Au NPs by 200-keV Xe impact. The NP radius is set to R=12.4 nm and the spherical cluster consists of 463,878 atoms. The Xe ion impacts on a local (111) facet. The local angle of incidence is varied between θ=0° (central impact) and 60°. In total, a number of 50 events are simulated. We follow the simulations for 100 ps.
The Au-Au interaction is modeled by a many-body potential which accurately reproduces the melting temperature of Au [18–20]. Note that the choice of the interaction potential is of prime importance for modeling sputtering phenomena under spike conditions [21–23]. Towards high energies, the potential has been splined to the Ziegler-Biersack-Littmark (ZBL) potential . The Xe ion interacts only by the repulsive ZBL potential with the Au atoms.
We model electronic stopping by a velocity-proportional friction force F=n k v, where n is the atomic number density of Au and v is the atom velocity. The constant k is taken from the Lindhard-Scharff formalism [25, 26], which gives k=0.506 eVÅps for the Au-Au and 0.388 eVÅps for the Xe-Au interaction. Usually, electronic stopping is not applied to slow atoms, with a kinetic energy below a cut-off, E c , since up-to-date estimates of electron-phonon coupling—which describes the low-energy transfer of electrons to atoms—give orders of magnitude smaller energy transfer than the Lindhard-Scharff prediction . While the exact value of E c is unknown—but expected to be in the range of a few eV [28, 29]—we adopt a value of E c =3.9 eV, equal to the cohesive energy; in collision-cascade sputtering, atoms with a smaller kinetic energy are never sputtered. For reference, we also performed a set of simulations for vanishing electronic losses. In order to investigate the role of electronic stopping in more detail, we performed further simulations with smaller E c , including E c =0 (where electron losses apply to all moving atoms in the NP), but only for perpendicular incidence.
We note, however, that all energy put into the electronic system of the NP will thermalize there and thus eventually flow back to the atomic system. This effect will raise the temperature of the NP after sputtering; we do not include this effect in our simulations presented here.
As a first orientation of the geometry of the energy deposition by the projectile in the NP, we use data of the range distribution provided by the SRIM software [30, 31] and corrected by the factors given in . This gives us the result that—in a bulk medium—the center of the deposited energy distribution is at a depth of a=19.9 nm below the surface; it has a longitudinal width of α=11.9 nm and a transverse width of β=11.1 nm. This means that the deposited-energy profile fills out the NP with radius R=12.4 nm, and hence, considerably more abundant sputtering is to be expected than from a semi-infinite flat target. In fact, recent calculations [13, 15] of the dependence of the sputter yield on the NP radius predict sputtering to become maximum when R≅a; this is the case here.
This figure shows that the NP is not filled homogeneously with energy by the projectile. This may appear astonishing since the dimensions of the deposited-energy ellipsoid are all comparable to the NP radius. However, it has been known for a long time that individual energy deposition profiles are actually smaller than the average deposited-energy ellipsoid , and our snapshots underline this fact for the present case.
We note that when electronic stopping is ignored, the temperature increase in the atomic system of the NP is higher (349 ± 49 K), since the spikes are longer lived, corresponding to 42 keV, while 158 keV leaves the NP by the transmitted projectile and the sputtered particles. Thus, electronic energy loss helps in localizing impact energy in the NP, since it is eventually refueled to the atomic system. This is a quite different situation from the bombardment of bulk targets, where the energy lost to the electronic system diffuses away.
We obtain an average sputter yield of 〈Y〉=397 ± 121 atoms. We also determined the sputter yield of a flat (infinitely thick) Au target under 200-keV Xe impact at normal incidence; it amounts to 116 ± 48 atoms.
This result can be compared with the experimental sputter yield of a flat surface. Szymczak and Wittmaack  measured Y=50 for (perpendicular) 200-keV Xe impact on a (111) Au surface. For comparison, we also note that the software TRIM (Transport of Ions in Matter)  gives a sputter yield of only 27 (Möller, W. Private communication 2014. Unpublished) for the flat surface; since TRIM takes only (ballistic) collision-cascade sputtering into account, this comparison demonstrates that spike sputtering is important already for the sputter emission from a bulk Au target.
The strong (fourfold) increase in sputter emission from the flat target to the NP target is similar to the data reported by Greaves et al.  for 80-keV Xe sputtering of Au nanorods. There, MD gave an average sputter yield of 1005. Only four individual experimental results are reported, ranging from 147 to 843.
Monte Carlo simulations show an increase of the sputter yield for nanospheres as compared to that of the bulk target . For the conditions of our system, a/R=0.623, these predict a yield enhancement of 6.98 for central impacts and of 2.14 as an average over all impacts. While these Monte Carlo simulations have been performed for another system (20-keV Ar on Si), they may be taken as a guideline to estimate the size of the ballistic enhancement effect to be expected. Our simulations show that the enhancement effect for collision spikes—here by a factor of around 4—may exceed that of collision-cascade sputtering.
Dependence of the sputter yield of a flat surface and a NP on the cut-off energy E c for electronic stopping. Data obtained for perpendicular incidence only
No electronic stopping
In experiment, NP sputtering is measured after depositing NPs on a substrate. In such a situation, the sputter yield will depend on the material of the substrate and the exact shape of the NP, which may vary depending on the deposition technique and the interface energy between NP and substrate from spherical over hemispherical to a flat layer. We estimate the sputter yield of a supported NP by assuming that only backsputtering contributes in this situation. Correcting the simulated sputter yield by excluding all forward-sputter events, we arrive at a sputter yield of 81 % of the total sputter yield, Y∼322 ± 98.
The experimental sputter yield of Au NPs under 200-keV Xe impact supported on a sapphire surface amounts to 149 ± 47 (Ziemann, P. Private communication 2010. Unpublished). The spherical particles were prepared by a self-assembly process leading to a narrow size distribution. The sputter yields were determined by monitoring the change of the particle size distribution on the surface as a function of ion fluence. The experimental sputter yield is slightly smaller than our MD estimate; including the theoretical and experimental error bars, the predictions are compatible with each other. Several reasons may contribute to this difference. (i) In the range of high temperatures and pressures and low particle densities relevant for the spike region, the interatomic potential is only poorly known; small changes in the interaction potential may affect the sputter yield in the spike regime [18, 28]. (ii) The role of the electronic system under spike conditions is complex. A recent model study  of spike sputtering of bulk Au targets showed that the energy loss to the electronic system will withdraw the energy from the atomic system; this may happen so rapidly that the collision spike may be quickly quenched and the sputter yield is reduced to that of the collision cascade. (iii) The interatomic interaction potential in Au depends on the electron temperature. A recent study  calculates this dependence and shows that in particular the melting temperature will be increased for high electron temperatures due to the increased electron pressure. It would be worthwhile to continue the present studies by including these coupled effects of the electron and atom system to the simulation of spike sputtering in NPs. (iv) The sputtering of a supported NP is a complex situation; on the one hand, energy can dissipate from the NP to the substrate decreasing the NP sputter yield; on the other hand, also the substrate may become sputtered and lead to a secondary sputtering of the NP. Such situations have up to now been rarely investigated . (v) Finally, artifacts in the experiment may affect the yield measurement. For example, it was recently reported  that even a single graphene layer on a metal surface decreases the sputter yield of metal atoms dramatically. If the NPs in the experiments were covered by a graphene (carbon) layer formed by the dissociation of ubiquitous hydrocarbons, this might have reduced the measured yield.
Ion irradiation of nanoparticles leads to enhanced sputter yields if the nanoparticle size is of the order of the ion penetration depth. While this feature is reasonably well understood for collision-cascade sputtering, we explore it in the regime of collision-spike sputtering using molecular-dynamics simulation. For the particular case of 200-keV Xe bombardment of Au particles, we show that collision spikes lead to abundant sputtering with an average yield of 397 ± 121 atoms compared to only 116 ± 48 atoms for a bulk Au target. Only around 31 % of the impact energy remains in the nanoparticles after impact; the remainder is transported away by the transmitted projectile and the ejecta. The sputter yield of supported nanoparticles will be only around 80 % of that of free nanoparticles due to the suppression of forward sputtering.
Simulation of NP sputtering is conceptually simpler than that of extended targets. Since electrons cannot escape the NP, the energy put by electronic stopping into the electronic system is not lost but remains in the target. Our simulations treat the system of 200-keV Xe impact on spherical Au NPs of R=12.4-nm radius as an exemplary case. In this case, the mean depth of energy deposition is situated almost in the center of the NP. Still, only around 20 % of the projectile energy is finally deposited in the NP; the remainder is transported away by the projectile and by the ejecta.
We find an average sputter yield of 397 ± 121, while the sputter yield of a bulk target is only 116 ± 48. Such large yields are due to spike effects which are virtually unquenched since electrons do not carry away the energy.
Around 20 % of the sputtered species is emitted in the forward direction. For supported NPs, this emission will be suppressed since the substrate will prevent ejection. The corresponding correction lowers the sputter yield to values of around 320.
Discussions with P. Ziemann are gratefully acknowledged. Part of the simulations were performed at the High Performance Cluster Elwetritsch (RHRK, TU Kaiserslautern, Germany). This work was partially performed under the auspices of the US Department of Energy by Lawrence Livermore National Laboratory and Los Alamos National Laboratory. LLNL is operated by Lawrence Livermore National Security, LLC, for the National Nuclear Security Administration of the U.S. DOE, under contract DE-AC52-07NA27344. LANL is operated by Los Alamos National Security, LLC, for the National Nuclear Security Administration of the U.S. DOE, under contract DE-AC52-O6NA25396.
- Krasheninnikov AV, Nordlund K. Ion and electron irradiation-induced effects in nanostructured materials. J Appl Phys. 2010; 107:071301.View ArticleGoogle Scholar
- Kirchner U, Vogt R, Natzeck C, Goschnick J. Single particle MS, SNMS, SIMS, XPS, and FTIR spectroscopic analysis of soot particles during the AIDA campaign. J Aerosol Sci. 2003; 34:1323.View ArticleGoogle Scholar
- Bringa EM, Kucheyev SO, Loeffler MJ, Baragiola RA, Tielens AGGM, Dai ZR, et al.Energetic processing of interstellar silicate grains by cosmic rays. Astrophys J. 2007; 662:372.View ArticleGoogle Scholar
- Bouchoule A. Dusty plasmas. Phys World. 1993; 6(8):47. No. 8.Google Scholar
- Järvi TT, Pohl D, Albe K, Rellinghaus B, Schultz L, Fassbender J, et al.From multiply twinned to fcc nanoparticles via irradiation-induced transient amorphization. Europhys Lett. 2009; 85:26001.View ArticleGoogle Scholar
- Klimmer A, Ziemann P, Biskupek J, Kaiser U, Flesch M. Size-dependent effect of ion bombardment on Au nanoparticles on top of various substrates: thermodynamically dominated capillary forces versus sputtering. Phys Rev B. 2009; 79:155427.View ArticleGoogle Scholar
- Greaves G, Hinks JA, Busby P, Mellors NJ, Ilinov A, Kuronen A, et al.Enhanced sputtering yields from single-ion impacts on gold nanorods. Phys Rev Lett. 2013; 111:065504. doi:10.1103/PhysRevLett.111.065504.View ArticleGoogle Scholar
- Yang L, Seah MP, Anstis EH, Gilmore IS, Lee JLS. Sputtering yields of gold nanoparticles by c60 ions. J Phys Chem C. 2012; 116:9311.View ArticleGoogle Scholar
- Kissel R, Urbassek HM. Sputtering from spherical Au clusters by energetic atom bombardment. Nucl Instrum Meth B. 2001; 180:293–8.View ArticleGoogle Scholar
- Kissel R, Urbassek HM. Sputtering of a Au surface covered with large spherical clusters. Int J Mass Spectrom. 2001; 208:29–35.View ArticleGoogle Scholar
- Zimmermann S, Urbassek HM. Sputtering of nanoparticles: molecular dynamics study of Au impact on 20 nm sized Au nanoparticles. Int J Mass Spectrom. 2008; 272:91–7. doi:10.1016/j.ijms.2008.01.004.View ArticleGoogle Scholar
- Järvi TT, Pakarinen JA, Kuronen A, Nordlund K. Enhanced sputtering from nanoparticles and thin films: size effects. Europhys Lett. 2008; 82:26002.View ArticleGoogle Scholar
- Järvi TT, Nordlund K. Sputtering of freestanding metal nanocrystals. Nucl Instrum Meth B. 2012; 272:66.View ArticleGoogle Scholar
- Nietiadi ML, Urbassek HM. Influence of local curvature on sputtering. Appl Phys Lett. 2013; 103:113108.View ArticleGoogle Scholar
- Nietiadi ML, Sandoval L, Urbassek HM, Möller W. Sputtering of Si nanospheres. Phys Rev B. 2014; 90:045417. doi:10.1103/PhysRevB.90.045417.View ArticleGoogle Scholar
- Sigmund P. Sputtering by ion bombardment: theoretical concepts In: Behrisch R, editor. Sputtering by Particle Bombardment I. Berlin: Springer: 1981. p. 9.Google Scholar
- Urbassek HM, Bradley RM, Nietiadi ML, Möller W. Sputter yield of curved surfaces. Phys Rev B. 2015; 91:165418. doi:10.1103/PhysRevB.91.165418.View ArticleGoogle Scholar
- Colla TJ, Urbassek HM. Au sputtering by cluster bombardment: a molecular-dynamics study. Nucl Instrum Meth B. 2000; 164-165:687–96.View ArticleGoogle Scholar
- Zimmermann S, Urbassek HM. Sputtering of Au (111) by 64 keV/atom Au clusters. Nucl Instrum Meth B. 2005; 228:75–83.View ArticleGoogle Scholar
- Zimmermann S, Urbassek HM. Sputtering of Au by cluster impact. Nucl Instrum Meth B. 2007; 255:208–13.View ArticleGoogle Scholar
- Urbassek HM. Molecular-dynamics simulation of sputtering. Nucl Instrum Meth B. 1997; 122:427–41.View ArticleGoogle Scholar
- Urbassek HM. Sputter theory In: Sigmund P, editor. Ion beam science: solved and unsolved problems. Mat. Fys. Medd. Dan. Vid. Selsk. vol. 52. Copenhagen: Royal Danish Academy of Sciences: 2006. p. 433–63.Google Scholar
- Urbassek HM. Results of molecular dynamics calculations In: Behrisch R, Eckstein W, editors. Sputtering by particle bombardment. Topics Appl. Physics. vol. 110. Berlin: Springer: 2007. p. 189–230.Google Scholar
- Ziegler JF, Biersack JP, Littmark U. The stopping and range of ions in solids. New York: Pergamon; 1985.Google Scholar
- Lindhard J, Scharff M. Energy dissipation by ions in the keV region. Phys Rev. 1961; 124:128.View ArticleGoogle Scholar
- Sigmund P, Bimbot R, Geissel H, Paul H, Schinner A. ICRU report 73: stopping of ions heavier than helium. J ICRU. 2005; 5(1):1–235. ICRU Report 73.View ArticleGoogle Scholar
- Sandoval L, Urbassek HM. Influence of electronic stopping on sputtering induced by cluster impact on metallic targets. Phys Rev B. 2009; 79:144115.View ArticleGoogle Scholar
- Samela J, Kotakoski J, Nordlund K, Keinonen J. A quantitative and comparative study of sputtering yields in Au. Nucl Instrum Meth B. 2005; 239:331.View ArticleGoogle Scholar
- Duffy DM, Rutherford AM. Including the effects of electronic stopping and electron-ion interactions in radiation damage simulations. J Phys: Condens Matter. 2007; 19:016207.Google Scholar
- Ziegler JF. SRIM. 2000. http://www.srim.org/.
- Ziegler JF. SRIM-2003. Nucl Instrum Meth B. 2004; 219-220:1027. SRIM: http://www.srim.org/.View ArticleGoogle Scholar
- Winterbon KB, Sigmund P, Sanders JB. Spatial distribution of energy deposited by atomic particles in elastic collisions. Mat Fys Medd K Dan Vidensk Selsk. 1970; 37(14):no. 14.Google Scholar
- Colla TJ, Aderjan R, Kissel R, Urbassek HM. Sputtering of Au (111) induced by 16-keV Au cluster bombardment: spikes, craters, late emission, and fluctuations. Phys Rev B. 2000; 62:8487–493. doi:10.1103/PhysRevB.62.8487.View ArticleGoogle Scholar
- Urbassek HM. Sputtering and laser ablation In: Hasselbrink E, Lundqvist BI, editors. Handbook of surface science vol. 3. Dynamics. Amsterdam: Elsevier: 2008. p. 871–913. Chap. 17.Google Scholar
- Anders C, Ziegenhain G, Ruestes CJ, Bringa EM, Urbassek HM. Crater formation by nanoparticle impact: contributions of gas, melt and plastic flow. New J Phys. 2012; 14:083016.View ArticleGoogle Scholar
- Westmoreland JE, Sigmund P. Correlation functions in the theory of atomic collision cascades: ion location and the distribution in depth and size of damage clusters. Radiat Eff. 1970; 6:187.View ArticleGoogle Scholar
- Szymczak W, Wittmaack K. Angular distributions of gold sputtered from a (111) crystal: dependence of spot shapes and of spot and background yields on the primary ion mass and energy and on the target temperature. Nucl Instrum Meth B. 1993; 82:220.View ArticleGoogle Scholar
- Biersack JP, Eckstein W. Sputtering studies with the Monte Carlo program TRIM,SP. Appl Phys A. 1984; 34:73.View ArticleGoogle Scholar
- Starikov SV, Stegailov VV, Norman GE, Fortov VE, Ishino M, Tanaka M. Laser ablation of gold: experiment and atomistic simulation. JETP Lett. 2011; 93:642.View ArticleGoogle Scholar
- Baranov I, Della-Negra S, Domaratsky V, Chemezov A, Novikov A, Obnorsky V, et al.Desorption of nanoclusters from gold nanodispersed layers by 72 keV Au 400 ions: experiment and molecular dynamics simulation. Nucl Instrum Meth B. 2008; 266:1993–2001.View ArticleGoogle Scholar
- Standop S, Lehtinen O, Herbig C, Lewes-Malandrakis G, Craes F, Kotakoski J. Ion impacts on graphene/Ir(111): interface channeling, vacancy funnels, and a nanomesh. Nano Lett. 2013; 13(5):1948–55.View ArticleGoogle Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.